| ||Format||Pages||Price|| |
|4||$41.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$41.00||  ADD TO CART|
|Standard + Redline PDF Bundle||8||$49.20||  ADD TO CART|
This specification covers the requirements for wrought cobalt-35nickel-20chromium-10molybdenum alloy for use in the manufacture of surgical implants. The alloy shall be manufactured into plates, sheets, and foils in the annealed, cold-worked, or cold-worked and capability-aged condition. The plates may be available in ground or dull finish, while the sheet and foil may be of dull cold-rolled, bright cold-rolled, intermediate polished, general-purpose polished, dull satin finished, high luster finish, or mirror finish. In addition, plate edges may be of rolled edge or approximate square edge, while for sheet and foil, edges may be approximate square edge or an edge produced by slitting or shearing. Heat and product analyses as well as tests for ultimate tensile strength, yield strength, elongation, hardness, and average grain size shall be performed and shall conform to the requirements specified.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers the chemical, mechanical, and metallurgical requirements for wrought cobalt-35nickel-20chromium-10molybdenum alloy (UNS R30035) in the form of plate, sheet, and foil to be used in the manufacture of surgical implants.
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with this standard.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E8/E8M Test Methods for Tension Testing of Metallic Materials
E10 Test Method for Brinell Hardness of Metallic Materials
E18 Test Methods for Rockwell Hardness of Metallic Materials
E29 Practice for Using Significant Digits in Test Data to Determine Conformance with Specifications
E112 Test Methods for Determining Average Grain Size
E140 Hardness Conversion Tables for Metals Relationship Among Brinell Hardness, Vickers Hardness, Rockwell Hardness, Superficial Hardness, Knoop Hardness, Scleroscope Hardness, and Leeb Hardness
E345 Test Methods of Tension Testing of Metallic Foil
E384 Test Method for Knoop and Vickers Hardness of Materials
F562 Specification for Wrought 35Cobalt-35Nickel-20Chromium-10Molybdenum Alloy for Surgical Implant Applications (UNS R30035)
F981 Practice for Assessment of Compatibility of Biomaterials for Surgical Implants with Respect to Effect of Materials on Muscle and Bone
ISO StandardsISO 9001 Quality Management Systems--Requirements Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org.
ICS Number Code 11.040.40 (Implants for surgery, prothetics and orthotics)
UNSPSC Code 42295500(Surgical implants and expanders and extenders and surgical wires and related products)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM F688-14, Standard Specification for Wrought Cobalt-35Nickel-20Chromium-10Molybdenum Alloy Plate, Sheet, and Foil for Surgical Implants (UNS R30035), ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top